Theoretical Investigation of Two-DimensionalSuperconductivity in Intercalated Graphene Layers
R. A. Jishi and D. M. Guzman
Department of Physics and Astronomy,
California State University, Los Angeles, California 90032, USA
H. M. Alyahyaei
Department of Physics and Astronomy,
University of California, Riverside, California 92521, USA
First-principles calculations of the electronic structure and vibrational modes, in
a system of graphene bilayers and trilayers intercalated with alkaline earth atoms,
are presented. It is found that, in similarity to the case of superconducting graphite
intercalation compounds, the Fermi level is crossed by an s-band derived from the
intercalant states, as well as graphitic -bands. The electron-phonon coupling pa-
rameter is found to be 0.60 and 0.80, respectively, in calcium intercalated graphene
bilayers and trilayers. In superconducting CaC6 graphite intercalation compound,
the calculated value for is 0.83. It is concluded that two-dimensional superconduc-
tivity is possible in a system of a few graphene layers intercalated with calcium.
PACS numbers: 71.15.Mb, 63.22.Rc, 73.22.Pr, 74.78.-w
Keywords: graphene intercalates, electron-phonon coupling, superconductivity
Superconductivity in graphite intercalation compounds (GICs) has been stud-ied extensively for a long period of time . A fascinating aspect of thesesuperconducting compounds is that they are usually formed from componentsneither one of which is a superconductor. In the case of alkali metal GICs thesuperconducting transition temperature is of the order of 1 K. Within the GICBrillouin zone (BZ) there exists an alkali-derived spherical band centered at the -point and carbon-derived cylindrical -bands centered along the HK axis. It wasproposed [6, 11, 12] that the presence of both bands is necessary for superconduc-tivity, and that a two-band model is capable of explaining various experimental
observations relating to the occurrence of superconductivity in alkali-metal GICsand their anisotropic magnetic properties.
It was also found that alkaline earth GICs exhibit superconductivity [7, 8] witha transition temperature of 6.5 K (YbC6) and 11.5 K (CaC6). Careful analysis of the electron-phonon coupling in CaC6 reveals that this superconductoris of the conventional BCS type, and that the presence of both Ca-derived andC-derived bands is necessary to explain the relatively high superconducting tran-sition temperature in this compound. It should be pointed out, however, thatsome controversy still exists regarding the mechanism for superconductivity inCaC6 GIC, whereas a large Ca isotope effect was measured in CaC6 GIC [17, 18]indicating a dominant role played by phonons due to Ca atomic vibrations, angle-resolved photoemission spectroscopy (ARPES) measurements on CaC6 GIC ,on the other hand, indicate that graphitic high frequency phonon modes are moststrongly coupled to electrons.
The recent discovery of stable graphene sheets  raises the question ofwhether two-dimensional superconductivity is possible in intercalated graphenelayers. The possibility of intercalating a system consisting of a few graphenelayers with intercalants, such as FeCl3 and Br, has been recently demonstrated[21, 22]. It is clear that a system consisting of many graphene layers, if inter-calated, should exhibit properties similar to those of GICs. It is natural to askwhether a system consisting of a few graphene layers, intercalated with alkali,or alkaline earth, metal atoms, will exhibit superconductivity. This problem wasdiscussed recently by Mazin and Balatsky , who considered a graphene bilayerintercalated with Ca. They argued, on the basis of similarities with the electronicenergy bands of the CaC6 GIC, that a graphene bilayer intercalated with Ca isprobably a superconductor.
In this paper we examine the problem of superconductivity in intercalatedgraphene layers. In particular, we calculate the energy bands in a graphene bi-layer intercalated with the alkaline earth atoms Ca, Sr, and Ba. In all three caseswe find that a band, derived from the alkaline earth atoms, crosses the Fermi en-ergy, along with carbon-derived -bands. We then calculate the electron-phononcoupling strength in these systems. The values obtained are reasonably large;in the case of Ca-intercalated bilayer, we find = 0.60, a value to be comparedwith 0.83 calculated in CaC6 GIC . Next, the case of a graphene trilayerintercalated with Ca is examined; here we find a value of 0.80 for the electron-phonon coupling strength . These calculations indicate that superconductivityis indeed possible in intercalated graphene layers.
In Section II we discuss the computational methods employed in this work.The results of the energy bands, vibrational modes, and electron-phonon couplingcalculations are presented and discussed in Section III, and conclusions are givenin Section IV.
The total energy and electronic band structure calculations are carried outusing the all-electron, full-potential, linear augmented plane wave (FP-LAPW)
method as implemented in the WIEN2K code . The exchange-correlationpotential was calculated using the generalized gradient approximation (GGA) asproposed by Pedrew, Burke, and Ernzerhof (PBE) . The radii of the muffin-tinspheres for the carbon and the alkaline earth atoms were taken as 1.3a0 and 2.5a0,respectively, where a0 is the Bohr radius. We set the parameter RMTKmax = 7,where RMT is the smallest muffin-tin radius and Kmax is a cutoff wave vector.The valence electrons wave functions inside the muffin-tin spheres are expandedin terms of spherical harmonics up to lmax = 10, and in terms of plane waveswith a wave vector cutoff Kmax in the interstitial region. The charge density isFourier expanded up to a maximum wave vector Gmax = 13a
10 . Convergence of
the self-consistent field calculations is attained with a total energy convergencetolerance of 0.01 mRy.
The calculations of the frequencies of the vibrational modes and the electron-phonon coupling parameter are performed using density functional theory (DFT)and ultrasoft pseudopotentials [27, 28]. The electron-phonon coupling strengthsare calculated using density functional perturbation theory within the linear re-sponse approximation. Ultrasoft pseudopotentials  are used for both, thealkaline earth and the carbon atoms. The valence electrons wave function andcharge density are expanded in plane waves using 30 Ry and 300 Ry cutoffs,respectively. In the calculation of the vibrational frequencies the electronic in-tegration is carried out using a uniform mesh of Nk = 8 8 k-points in thetwo-dimensional BZ. On the other hand, the electronic density of states, used incomputing the electron-phonon coupling parameter , is calculated using a fineruniform mesh of 24 24 k-points. The value of is obtained by averaging overa uniform mesh of Nq = 6 6 phonon momentum q-points.
III. RESULTS AND DISCUSSION
The first issue to decide is this: given a graphene bilayer, will it be energeticallyfavorable for the alkaline earth atoms to be intercalated between the two carbonsheets comprising the bilayer? Or will the energy be lower if the alkaline earthatoms sit on top of the bilayer? If the atoms sit on top of the bilayer, the resultingstructure will be denoted by C6-C6-A, where A represents an alkaline earth atom.On the other hand, the intercalated structure is denoted by C6-A-C6. In orderto decide which structure is more stable, we carried out total energy calculationsfor both structures. In the case of C6-C6-A, the alkaline earth atom is placedover the center of a hexagon in the upper sheet, and its distance to the sheet isvaried in order to find the lowest energy. On other hand, in the case of C6-A-C6, the distance between the carbon sheets is fixed at the measured separationin the corresponding graphite intercalation compound [9, 30]. In all the casesconsidered, corresponding to A=Ca, Sr, and Ba, we found that the energy is lowerfor the intercalated structure. For the case A=Ca, the intercalated structure C6-Ca-C6 is lower in energy than the C6-C6-Ca structure by 0.47 eV/Ca atom. In theother two cases, A=Sr and Ba, the energy of the C6-A-C6 structure is lower thanthe C6-C6-A structure by 0.43 eV/Sr atom and 0.59 eV/Ba atom. We concludethat it is energetically favorable for the alkaline earth atom to be intercalated in
between the graphene layers.
FIG. 1: (Color online) (a) The unit cell of the structure C6-A-C6, where A is an alkaline
earth atom, is shown. (b) The 2-D Brillouin zone of a graphene layer (or bilayer) is
shown as a dashed hexagon, while that for the intercalated graphene bilayer is shown
as a solid hexagon. Note that the M and K points in the graphene BZ (here denoted
by M and K) are folded onto points M and , respectively, of the intercalated bilayer
In the following we focus attention only on the C6-A-C6 structure. The sepa-ration between the two carbon sheets of the intercalated bilayer is taken as 4.52A, 4.94 A, and 5.25 A for A=Ca, Sr, and Ba, respectively. The unit cell is a(
3a) R 30 supercell of the graphene sheet unit cell; i.e., the in-planelattice constant of C6-A-C6
Click here to load reader